advertisement

Spectral dependence of the magnetic modulation of surface plasmon polaritons in noble/ferromagnetic/noble metal films The MIT Faculty has made this article openly available. Please share how this access benefits you. Your story matters. Citation Martín-Becerra, Diana et al. “Spectral Dependence of the Magnetic Modulation of Surface Plasmon Polaritons in Noble/ferromagnetic/noble Metal Films.” Physical Review B 86.3 (2012): 035118. © 2012 American Physical Society. As Published http://dx.doi.org/10.1103/PhysRevB.86.035118 Publisher American Physical Society Version Final published version Accessed Fri May 27 00:31:21 EDT 2016 Citable Link http://hdl.handle.net/1721.1/72207 Terms of Use Article is made available in accordance with the publisher's policy and may be subject to US copyright law. Please refer to the publisher's site for terms of use. Detailed Terms PHYSICAL REVIEW B 86, 035118 (2012) Spectral dependence of the magnetic modulation of surface plasmon polaritons in noble/ferromagnetic/noble metal films Diana Martı́n-Becerra,1,* Vasily V. Temnov,2,† Tim Thomay,3,‡ Alfred Leitenstorfer,3 Rudolf Bratschitsch,3,§ Gaspar Armelles,1 Antonio Garcı́a-Martı́n,1 and Marı́a Ujué González1, 1 IMM-Instituto de Microelectrónica de Madrid (CNM-CSIC), Isaac Newton 8, PTM, E-28760 Tres Cantos, Madrid, Spain 2 Department of Chemistry, Massachusetts Institute of Technology, Cambridge, Massachusetts 02139, USA 3 Department of Physics and Center for Applied Photonics, University of Konstanz, D-78457 Konstanz, Germany (Received 21 March 2012; revised manuscript received 1 June 2012; published 12 July 2012) The magnetic ﬁeld is an interesting candidate for the development of active plasmonic devices as it is able to modify the surface plasmon polariton (SPP) wave vector. Both real and imaginary parts of the SPP wave vector are affected. Here, we have experimentally determined the contribution of both modulations in the spectral range λ0 = 500–1000 nm for magnetoplasmonic systems consisting of noble/ferromagnetic/noble multilayered metal ﬁlms. We have seen that the real part usually exceeds the imaginary one, but in the longer wavelength range the contribution of the imaginary part cannot be neglected. We have analyzed the spectral dependency of the modulation, and we conclude that it is dominated by the evolution of the SPP properties with wavelength and not the magneto-optical parameter. A ﬁgure of merit including modulation and propagation distance is also studied for the three ferromagnetic metals, Fe, Co, and Ni. DOI: 10.1103/PhysRevB.86.035118 PACS number(s): 75.70.Cn, 71.36.+c, 73.21.Ac, 73.20.Mf I. INTRODUCTION The increasing demand of our society for faster communication networks and information-processing systems, being at the same time more efﬁcient or greener in terms of energy consumption, constitutes a key driving force towards the progress of integrated photonic devices. The design and fabrication of new nanoscale optical systems becomes therefore crucial in order to deliver all the different functions required in these devices. Surface plasmon polaritons (SPPs) are propagating electromagnetic waves bound to a metaldielectric interface, therefore vertically conﬁned. Besides, they can be laterally conﬁned beyond the diffraction limit by nanostructuring the interface. Recent advances in SPP-based (plasmonic) systems, with a wide range of passive coupling and guiding elements demonstrated, show that they are one of the relevant candidates to achieve these nanophotonic circuits,1–4 provided that the intrinsic loss of the system can be overcome by using appropriate gain strategies.5 Furthermore, important progress has been made in the last years to achieve active plasmonic conﬁgurations,6–18 i.e., plasmonic systems that could be externally manipulated, which is a critical step to really endow plasmonic systems with full capacity of development of nanophotonic chips as it will allow the realization of fundamental components such as modulators, switches or active multiplexors, couplers, and add-drop ﬁlters. Several external agents have been proposed so far to provide the controlled response of these active plasmonic systems: temperature,6,7,14 voltage,10,11,17,18 optical signals,8,9,12,13 or magnetic ﬁeld.15,16 In all cases, the mechanism underlying the modiﬁcation of the system’s response is either the control of absorption6,8,9,11,17 or the modiﬁcation of the material refractive index and thus of the SPP wave vector7,10,14–16,18 (a combination of both in some speciﬁc cases12,13 ). The use of magnetic ﬁeld and associated magneto-optical (MO) effects as the driving agent can be of particular interest because of its ﬂexibility. It has been known since the early seventies that a magnetic ﬁeld B = B0 x̂ parallel to the interface 1098-0121/2012/86(3)/035118(7) induces a modiﬁcation on the wave vector of a SPP traveling in the perpendicular direction, ksp = ksp ŷ [see sketch in Fig. 1(a) for relative directions]:19–21 0 ksp (±B0 ) = ksp ± ksp (B0 ), (1) 0 is the SPP wave vector without applied magnetic where ksp ﬁeld and ksp is the modulation induced by the magnetic ﬁeld, which is related to the off-diagonal element of the dielectric tensor yz , also called MO constant. This modiﬁcation occurs r r i in both the real and imaginary part of ksp : ksp (ksp ) and ksp i (ksp ), respectively. The amount of modulation of each part is different, and is a function of the optical and MO properties of our particular system. The real and imaginary parts of ksp r represent different physical properties: ksp accounts for the i SPP phase velocity while ksp is related to its propagation distance. Therefore, the magnetic ﬁeld offers the opportunity of designing active plasmonic systems based on the control i dominates, or on effective refractive of absorption if ksp r index modiﬁcation if ksp does. Moreover, as can be seen in Eq. (1), the SPP modiﬁcation under an applied magnetic ﬁeld is nonreciprocal [ksp (B0 ) = −ksp (B0 )], thus making this kind of system very interesting for the design of integrated optical isolators,22–26 another fundamental piece for the development of nanophotonic circuits. Another advantage of the magnetic ﬁeld driven systems is related to its potential switching speed, as it has been recently demonstrated that materials magnetization switching is an ultrafast phenomenon that can achieve the terahertz regime.27 The implementation of magnetic ﬁeld induced modulation on plasmonic systems in the optical regime requires the use of materials combining good properties in terms of plasmon propagation and MO constant of sizable value. Unfortunately, noble metals have a quite small MO constant, so a magnetic material has to be introduced in the system to increase this response. Ferromagnetic metals seem an appropriate choice as they also support plasmons due to their metallic nature; however, their high optical absorption induces an excessive 035118-1 ©2012 American Physical Society DIANA MARTÍN-BECERRA et al. PHYSICAL REVIEW B 86, 035118 (2012) spreading of the evanescent wave. Finally we discuss the optimum spectral range for application purposes in terms of a ﬁgure of merit combining both modulation and SPP propagation distance. (a) r i II. EXPERIMENTAL DETERMINATION OF ksp AND ksp (b) FIG. 1. (Color online) (a) Left side: Sketch of the magnetoplasmonic interferometer with deﬁnition of the system geometry and structural parameters. Right side: Image from the slit back side, showing the transmitted intensity interference pattern resulting from the interference between the light directly transmitted through the slit and the surface plasmon polariton excited at the groove and decoupled at the slit after having traveled the groove-slit distance. (b) Optical (top panel) and magnetoplasmonic (bottom panel) interferograms for an interferometer with the following particular geometry: slit-groove angle θ = 5◦ , minimum slit-groove distance d(0) = 20 μm, AuCoAu trilayer of h = 25 nm. The measurements correspond to λ0 = 633 nm. The right side inset shows a zoomed portion of both interferometers to depict in more detail the phase shift, φ. damping of the SPP propagation which prevents their use as the only metallic component of the system. This has led to the combination of noble and ferromagnetic metals as suitable magnetoplasmonic systems.15,16,28–31 The possibility of realizing magnetic ﬁeld driven SPP modulators has been recently demonstrated using this kind of system.15 Moreover, the modulation can be increased with the addition of a thin dielectric layer on top of the metallic multilayer,16 or by optimizing the quality of the interfaces.31 A deeper understanding of the behavior of these systems would allow for a further development of active plasmonic devices acting through a magnetic ﬁeld. In this paper, we have experimentally determined the spectral evolution of the modulation of both the real and imaginary parts of the SPP wave vector in the visible and nearinfrared (from 500 nm to 1 μm) for Au/Co/Au multilayered systems. As will be shown, the relative weight of each part depends on the wavelength range, so this aspect has to be taken into account to optimize the obtained response in these systems. We also analyze the dependence of both modulations on the different optical and magneto-optical parameters of the system, expanding the study to other ferromagnetic metals. We have found that the spectral behavior of ksp is dominated by the evolution of the SPP properties, namely the vertical The values of the real and imaginary part of the SPP wave vector modulation induced by the magnetic ﬁeld have been obtained by means of plasmonic microinterferometry with tilted groove-slit arrangement,13 using the same conﬁguration as that employed for the implementation of magnetoplasmonic modulators.15,16 A sketch of this conﬁguration is shown in Fig. 1(a): A slit and a tilted groove have been engraved by means of a focused ion beam (FIB) on a Au/Co/Au trilayer (total thickness 200 nm). The thickness of the Co layer, tCo , is 6 nm, and it is placed at different depths from the trilayer surface (h = 15, 25, and 35 nm). The slit, of width 100 nm, goes through all the metal thickness, while the groove, 200 nm wide, has a depth of around 100 nm. These dimensions, although not optimized for maximum coupling or resonant transmission of SPPs at each wavelength,32 have allowed us to satisfactorily excite and detect the surface plasmon polaritons in all the aimed spectral range, from 500 nm to 1 μm. When illuminating the interferometer with a p-polarized laser beam, the light collected at the back side of the slit results from the interference between light directly transmitted through the slit and light originating from a surface plasmon polariton that has been excited at the groove, has traveled towards the slit, and is decoupled in the slit. This transmitted light intensity can be expressed as r I = A2r + A2sp (x) + 2Ar Asp (x) cos ksp d(x) + ϕ0 , (2) where Ar corresponds to the ﬁeld amplitude of the light passing directly across the slit and Asp to that associated with the SPP. Due to the tilted groove-slit conﬁguration, the distance d between them depends on the position along the slit, d(x), and the optical path difference entering in the cosine argument changes, which results in a pronounced interference pattern along the slit axes, as can be seen in Fig. 1(a). The SPP related ﬁeld amplitude Asp also depends on d(x) because of i g the damping during SPP propagation, Asp (x) = Asp e−ksp d(x) , g where Asp is the amplitude of the excited SPP at the groove position, which in principle is, as Ar , constant along the groove. The phase ϕ0 is a constant phase arising during SPP coupling at the groove and uncoupling at the slit. We collect the intensity at the back side of the slit by scanning a photodiode along a projected image obtained with a 20× long-distance objective. This signal constitutes the optical interferogram, and an example corresponding to an interferometer with slit-groove angle θ = 5◦ and minimum slit-groove distance d(0) = 20 μm in a AuCoAu trilayer of h = 25 nm, measured at λ0 = 633 nm, is plotted in the top panel of Fig. 1(b). If an external periodic (1.4 kHz in our experimental conﬁguration) magnetic ﬁeld high enough to saturate the sample (B ≈ 20 mT) is applied parallel to the sample interface and along the slit axis, a modiﬁcation in the SPP wave vector is induced following Eq. (1), which results in a modiﬁcation of the optical path difference and therefore a shift in the interference pattern. This leads to a variation of the transmitted 035118-2 SPECTRAL DEPENDENCE OF THE MAGNETIC . . . PHYSICAL REVIEW B 86, 035118 (2012) intensity at each point of the slit synchronous with the applied magnetic ﬁeld, I = I (+M) − I (−M) ≡ Imp . In a ﬁrst-order approximation, this intensity variation corresponds to the derivative of the transmitted intensity I with respect to the magnetic ﬁeld, and it can be expressed as r 2 + k i 2 sin k 0r d + ϕ + φ , Imp = −4Ar Asp d ksp 0 sp sp (3) 0r ksp 0i ksp and are the real and imaginary parts of ksp when where there is no magnetic ﬁeld applied. This intensity variation is collected with the scanning photodiode by using lock-in detection and constitutes the magnetoplasmonic interferogram [see bottom panel of Fig. 1(b)]. It can be seen that Imp is proportional to the modulus of ksp and to the distance covered by the plasmon d. Moreover, Imp is phase shifted r with respect to I : The modulation of ksp induces a π/2-phase i shift, and the presence of ksp adds an additional φ phase, i r deﬁned as tan φ = ksp /ksp [a full derivative of Eq. (3), r i with the explicit contribution of ksp and ksp , can be found in the Appendix]. By determining the phase shift between both interferograms and the ratio of the amplitude of the magnetoplasmonic signal to the amplitude contrast of the optical one [shown in Fig. 1(b)], both the real and imaginary parts of the SPP wave vector modulation can be determined. r i as dashed lines, the values of ksp and ksp obtained from numerical simulations performed in the following way:33 Our multilayered air/Au/Co/Au/glass system is modeled by means of a transfer matrix formalism where the magneto-optical activity is accounted for by describing the Co layer with the corresponding dielectric tensor. Then, a numerical solver for guided modes is applied to ﬁnd the SPP supported by the metal-air interface in the presence and absence of an applied magnetic ﬁeld B. The optical and MO constants of the different materials involved have been obtained by ellipsometric and polar Kerr characterization,29 respectively, of the samples containing the interferometers. As can be seen, the agreement between the experiment and the simulations is very good. As Fig. 2 shows, the general trend for both real and imaginary part wave vector modulations is that the modulation value decreases with wavelength, an unexpected behavior in principle as the absolute value of the MO constants of Co increase with wavelength [see Fig. 3(a)], and whose origin will be discussed in detail in the next section. The same behavior is obtained for all three different positions of the Co layer, (a) r i III. SPECTRAL BEHAVIOR OF ksp AND ksp (b) In order to analyze their spectral dependence, we have mear i sured ksp and ksp by illuminating the magnetoplasmonic interferometers with several lasers of different wavelengths (λ0 = 532, 633, 680, 785, 860, and 890 nm). The obtained results are plotted in Fig. 2 (ﬁlled symbols) for three trilayers where the Co layer is placed at different positions, h = 15, 25, and 35 nm. The upper graph corresponds to the real part of the modulation, and the lower graph to the imaginary part. Together with the experimental results, Fig. 2 also includes, r FIG. 2. (Color online) Wavelength dependence of ksp (top i (bottom graph) obtained for magnetoplasmonic graph) and ksp trilayers with three different positions of the Co layer, h = 15, 25, and 35 nm. The ﬁlled symbols correspond to experimental values and the dashed lines to values obtained numerically. The inset shows the i r /ksp , which corresponds to tan φ. calculated ratio ksp (c) FIG. 3. (Color online) (a) Wavelength dependence of the magneto-optical parameter Q for our Co layers, as obtained from ellipsometric and polar Kerr characterization. (b) Evolution of the plasmonic term from the analytical expression of ksp for the AuCoAu trilayers. Both the long-wavelength approximation (real part in black dash-dot line and imaginary part in dashed red line) and complete expressions (real part in black solid line and imaginary part in dotted red line) are plotted. (c) Spectral dependence of the intensity of the SPP magnetic ﬁeld at the middle of the Co layer in a AuCoAu trilayer with h = 15 nm. The SPP magnetic ﬁeld intensity is normalized in such a way that the intensity integrated along the z axis is 1 for each wavelength. (d) Evolution with wavelength of the separation of the SPP wave vector from the light line (left axis; real part in black solid line and imaginary part in red dotted line) compared with the evolution of ksp (right axis; real part in black dash-dot line and imaginary part in dashed red line) for a AuCoAu trilayer (in particular, the case for h = 15 nm is plotted). 035118-3 DIANA MARTÍN-BECERRA et al. PHYSICAL REVIEW B 86, 035118 (2012) with the only difference of getting smaller absolute values of modulation as the Co layer lies deeper in the trilayer. This is due to the evanescent nature of the SPP: Its electromagnetic ﬁeld decays exponentially inside the metal, and therefore the deeper the Co (ferromagnetic) layer the less electromagnetic ﬁeld and as a consequence the less magnetic modulation would be achieved.15 Regarding the real part of ksp , it presents a peak at low wavelengths (λ0 = 530 nm).34 This peak is not associated with a resonant behavior but with the presence of absorption in the metal, which makes the SPP dispersion relation bend around this wavelength close to the surface plasmon resonance frequency35 (the discussion in the next section will clarify this point). As for the imaginary part, it is in general smaller than the real part in most of the spectral range. Only in the smallest wavelength part (λ0 < 520 nm), again close to the surface plasmon resonance frequency, the imaginary part dominates. At this wavelength range, there is a discrepancy between theory and experiment, mainly due to the very short SPP propagation distance, which worsened signiﬁcantly the signal-to-noise ratio during experiment. Taking into account the ratio between imaginary and real part modulations, shown in the inset included in Fig. 2, three spectral regions can be deﬁned. For lower wavelengths (λ0 < 520 nm), the dominant part of the modulation is the imaginary one, but this is a region where plasmon losses are too high to envisage any practical application of these systems. For the central range, between λ0 = 550 nm and around 750 nm, the relevant component of the modulation is the real part, the imaginary one being a small perturbation that can be discarded (tan φ ≈ 0), as was done in previous studies of the magnetoplasmonic modulators.15,16 Finally, for the long-wavelength region the ratio increases, so that the imaginary part has to be taken into account in order to accurately describe the system. For example, in magnetoplasmonic modulators implemented in the form of interferometers and therefore based on the intensity variation i given by Eq. (3), the contribution of ksp is important to ﬁnd the slit-groove distance of maximum response, as φ can no longer be neglected. IV. DISCUSSION ON THE DIFFERENT FACTORS GOVERNING ksp To gain a deeper understanding on the obtained spectral behavior of the modulation of ksp , an equation relating the implied parameters is necessary. An analytical expression for ksp in a noble/ferromagnetic/noble metal trilayer can be obtained considering that the ferromagnetic layer (Co here) is very thin and that the MO activity is a small perturbation in the system (|yz | |xx |):15 2 k02 d2 Au Au × QCo , ksp ≈ 2tCo e−2hkz × 2 2 d − Au d + Au (4) where tCo and h are the thickness and depth of the Co layer, respectively; kzAu is the z component of the SPP wave vector inside the metal; Au and d are the dielectric constants of Au and of the dielectric medium on top of the metallic trilayer; 0 corresponds k0 is the wave vector of light in vacuum; ksp to the SPP wave vector of a semi-inﬁnite metal-dielectric interface;35 and QCo is the Co magneto-optical parameter. To get an insight on the main parameters governing ksp behavior, we can also employ the following approximation valid in the long-wavelength regime (d Au ): k02 d2 × QCo Au ≡ Astr × B plasm × QCo . ksp ≈ −2tCo e−2hkz × Au (5) We can split both Eqs. (4) and (5) into three terms: a structural term Astr , a purely optical or plasmonic term B plasm , and a MO term QCo . The structural term Astr is governed by geometric parameters regarding the structure (tCo and h) and the z component of the SPP wave vector inside the metal, kzAu , which is also associated with the exponential decay of the SPP electromagnetic ﬁeld intensity inside the metal layer mentioned before hardly depends on the wavelength, so it will not be further taken into account. The plasmonic term B plasm includes all the optical parameters of the system except for those related to the ferromagnetic layer: Au , d (1 in the case analyzed here), and k0 . Thus, this term takes into account the properties of the surface plasmon polariton supported by the system for each wavelength. Finally, the MO properties of our ferromagnetic layer appear in the last term through the Co Co magneto-optical parameter Q, deﬁned as QCo = iyz /xx Co Co (for xx and yz the optical and magneto-optical constants of Co, respectively). The spectral behavior of ksp is therefore determined by QCo and B plasm , whose dependencies on the wavelength are plotted in Figs. 3(a) and 3(b), respectively. Figure 3(b) shows the plasmonic term in the exact expression of Eq. (4) as well as the long-wavelength approximation [Eq. (5)]. As can be seen, the approximation is very good beyond 700 nm. From the results plotted in Figs. 3(a) and 3(b) we can establish that the spectral behavior of ksp in our AuCoAu magnetoplasmonic multilayers is dominated by the plasmonic term: The absolute value of Q increases with the wavelength while the plasmonic term shows the same decreasing behavior as ksp as well as the presence of a small peak in the real part for small wavelengths. This shows that the evolution of the SPP properties with the wavelength is very important to determine the possible magnetic modulation achieved. A signiﬁcant SPP property is the SPP ﬁeld vertical spreading, which affects the amount of ﬁeld reaching the ferromagnetic layer. Actually, it has already been demonstrated that when covering the metallic multilayers with dielectric ﬁlms of different thickness, the magnetic ﬁeld induced modulation of the SPP wave vector evolves in the same way as the redistribution of the SPP electromagnetic ﬁeld.16 The same mechanism, as a function of the wavelength, can be invoked here. In fact, we can rewrite Eq. (4) so that the amount of SPP ﬁeld inside the Co layer appears explicitly. For that, we refer to the SPP magnetic ﬁeld component intensity |Hy |2 at the Co layer position. This magnitude is normalized so that for each wavelength the integral of |Hy |2 along the z axis is equal to 1 (the energy density is the same in all cases). Taking into account that for a Au/dielectric semi-inﬁnite interface the normalized SPP magnetic ﬁeld can Au be written as [2kzAu kzd /(kzAu + kzd )]1/2 e−kz z , with kzAu and kzd the z components of the SPP wave vector in the metal and 035118-4 SPECTRAL DEPENDENCE OF THE MAGNETIC . . . PHYSICAL REVIEW B 86, 035118 (2012) dielectric, respectively, and using some arithmetic, we obtain the following expression: √ k0 d Au −(d + Au ) Co 2 Hy ksp ≈ tCo × × QCo . (6) 2 d2 − Au In Fig. 3(c), we plot |HyCo |2 as a function of the wavelength. The SPP ﬁeld does indeed decrease with the wavelength, as ksp does, conﬁrming that the penetration of the SPP in the MO layer is the main parameter to take into account in the spectral behavior of ksp . The SPP ﬁeld, however, does not reproduce all the details found in the spectral evolution of r i ksp and ksp . This is due to the inﬂuence of other optical parameters, as can be seen from Eq. (6). The term containing the proportionality to the SPP ﬁeld at the Co layer interface contains some other optical factors whose particular spectral response slightly modiﬁes the pure decay of the ﬁeld with the wavelength, to ﬁnally deﬁne the obtained spectral shape of ksp (real and imaginary parts). This information on the spectral dependence of SPP electromagnetic ﬁeld conﬁnement, implicit in B plasm , is also contained in the dispersion relation. If we consider the sepa0 ration of the SPP wave vector from the light line, ksp − k0 , the bigger separation occurring at shorter wavelengths implies a stronger evanescent decay and therefore a higher conﬁnement. 0 As a consequence, the magnitude ksp − k0 is also able to describe the spectral shape of ksp , and we have found that r i it does it in a very accurate way for both ksp and ksp for our AuCoAu trilayered system, as shown in Fig. 3(d). Summarizing, for longer wavelengths the SPP wave vector is closer to the light line and thus the associated electromagnetic ﬁeld is more spread out of the interface, while for smaller wavelengths ksp increases and the SPP ﬁeld becomes more conﬁned to the interface and the presence of the Co layer is strongly felt. Our results show that this effect has a bigger inﬂuence on ksp than the increase of QCo with wavelength. V. EXTENSION TO OTHER FERROMAGNETIC METALS The discussion performed above regarding the spectral evolution of the magnetic ﬁeld driven modulation of SPP wave vector for the particular AuCoAu trilayer system could be, in principle, extended to the other ferromagnetic metals, Fe and Ni, as the different parameters, ksp properties and Q, evolve in a similar way. The right axis of Fig. 4(b) r i shows the calculated values of ksp and ksp for trilayers of Au/FerromagneticMetal/Au with a ferromagnetic metal layer of 6 nm and h = 15 nm. To make the analysis as general as possible, instead of employing optical and MO dielectric constants experimentally determined in our laboratory, we have chosen in this case to use well-established values that can be found in the literature for the bulk forms of the analyzed materials: Au, dielectric constant;36 Fe and Co, optical37 and MO38 constants; and Ni, optical39 and MO40 constants. In Fig. 4(a), the corresponding magneto-optical parameters Q for Fe, Co, and Ni are shown. As can be seen in Fig. 4(b), the greatest absolute values of modulation are obtained for Fe, and Ni provides the lowest values, in agreement with the values of Q parameter for each metal. Regarding the evolution with wavelength, ksp behaves in the expected decreasing way, (a) (b) FIG. 4. (Color online) (a) Wavelength dependence of the magneto-optical parameter Q for the three ferromagnetic metals Fe (dotted green line), Co (solid black line), and Ni (blue dashed line), calculated from typical optical and magneto-optical constants for the Fe Fe (Ref. 37), yz (Ref. 38), bulk materials referred to in the literature: xx Co Co Ni Ni xx (Ref. 37), yz (Ref. 38), xx (Ref. 39), and yz (Ref. 40). (b) Right axis: Dependence on wavelength of the real part (black dash-dot line) and the imaginary part (red dashed line) of calculated ksp for trilayers of Au/FerromagneticMetal/Au with h = 15 nm and tFerro = 6 nm, where Fe (top panel), Co (middle panel), and Ni (bottom panel) are the ferromagnetic metal. Left axis: Comparison of the calculated ksp with the separation of the SPP wave vector from the light line (real part in black solid line and imaginary part in red dotted line). The Q parameter used in the calculations is the one shown in part (a) of the ﬁgure. even for increasing values of Q, conﬁrming the predominance of the plasmonic term to determine this evolution. Figure 4(b) 0 also compares the evolution of ksp with the distance of ksp to the light line (left axis), with again a good agreement between both quantities. The matching between ksp and 0 ksp − k0 trends is slightly worse in the case of Fe, mainly at small wavelengths, because of the stronger dependency of QFe with wavelength in this regime, which gives rise to a stronger convolution of the product of the MO and the plasmonic term in Eq. (5) for this ferromagnetic metal. It is well known that the propagation distance of surface plasmon polaritons increases with wavelength, so that longer wavelengths would provide a higher ﬂexibility in the design of magnetic ﬁeld driven plasmonic devices. For example, in the case of magnetoplasmonic modulators based on interferometers, the modulated intensity Imp is proportional to the product of ksp times the slit-groove distance d,15,16 so that higher modulations can be obtained by increasing this distance. Therefore, in order to evaluate the optimal spectral range for the performance of magnetoplasmonic modulators, the 035118-5 DIANA MARTÍN-BECERRA et al. PHYSICAL REVIEW B 86, 035118 (2012) FIG. 5. (Color online) Spectral evolution of the ﬁgure of merit r )2 + (k i )2 × L for the same Au/FerromagneticMetal/Au (ksp sp sp trilayers as in Fig. 4, with the ferromagnetic metal being Fe (dotted green line), Co (solid black line), and Ni (blue dashed line). √ r 2 i 2 product (ksp ) + (ksp ) × Lsp , with Lsp being the length at which the surface plasmon polariton intensity decays a factor 1/e, constitutes an adequate ﬁgure of merit.16 Figure 5 shows this ﬁgure of merit for the three Au/FerromagneticMetal/Au trilayers with Fe, Co, and Ni. The best performance in absolute terms is again obtained by Fe, Ni being the worst one, in agreement with the amount of MO response strength as i r > ksp , indicated by Q. In the wavelength region with ksp λ0 < 520 nm, the ﬁgure of merit is too small since the propagation distance of the SPP is almost zero. In the spectral range where SPPs start having propagation distances of a few microns and therefore could be employed in photonic devices (SPP propagation distance Lsp > 3 μm at λ0 > 600 nm for a Au/Co/Au trilayer with the Co layer placed at h = 15 nm), the ﬁgure of merit increases and achieves its maximum value at around 1 μm. At these wavelengths, as was seen from Fig. 2, both real and imaginary components of the modulation are relevant. Finally, for wavelengths λ0 > 1 μm, the ﬁgure of merit decreases a little, seeming to reach a saturation value. Taking the values of Fig. 5 into consideration, a magnetoplasmonic modulator consisting of a Au/Fe/Au interferometer with a separation distance of 3Lsp (achievable from our experimental experience) and covered with a dielectric with εd = 2 (see Ref. 16) could provide intensity modulations (I /I = 2|k|Lsp )15 of around 12% in the optimal spectral range (950 nm). This value is not far from other integrated plasmonic modulator performances reported in the literature based on thermo-optical or electro-optical effects.14,18 These examples have the advantage of being already implemented in SPP waveguide conﬁgurations, while the interferometer geometry is still an extended one. However, magneto-optical effects offer the advantage of higher switching speed. VI. CONCLUSIONS We have determined both the real and the imaginary parts of the magnetic ﬁeld induced modiﬁcation of the SPP wavevector for Au/FerromagneticMetal/Au magnetoplasmonic systems. It has been shown that the real part is the dominating component in most of the spectral range, although at longer wavelengths the values of both components approach and the imaginary part has to be taken into account to appropriately describe the system response. The spectral dependence of the SPP wave vector modulation has been characterized, and it shows a decreasing behavior with wavelength. By means of an analytical expression for ksp obtained in the approximation of a very thin ferromagnetic metal layer, we have established that this spectral trend is due to the evolution of the SPP properties with wavelength. These properties come from the vertical conﬁnement of the SPP ﬁeld, which can be qualitatively described by the evolution of the separation between the SPP wave vector and the light line. The spectral behavior has been also calculated for Fe and Ni, evolving the same way as for Co. A ﬁgure of merit combining both magnetic modulation and propagation of the SPP is also analyzed. In terms of spectral dependence, the decrease of SPP wave vector modulation is overcompensated by the increase in Lsp for a signiﬁcant wavelength range, so that the 700 nm to 1 μm interval becomes the optimal one. ACKNOWLEDGMENTS We acknowledge funding from the EU (NMP3-SL2008-214107-Nanomagma), the Spanish MICINN (“MAPS” MAT2011-29194-C02-01, “MAGPLAS” MAT2008-06765C02-01/NAN, and “FUNCOAT” CONSOLIDER INGENIO 2010 CSD2008-00023), the Comunidad de Madrid (“MICROSERES-CM” S2009/TIC-1476), and Deutsche Forschungsgemeinschaft and Region Pays de La Loire. APPENDIX: DERIVATION OF THE MAGNETOPLASMONIC INTERFEROGRAM EQUATION When we apply a magnetic ﬁeld, a variation of the transmitted intensity at each point of the slit associated with the modulation of the SPP wave vector takes place: I = I (+M) − I (−M) ≡ Imp . In a ﬁrst-order approximation (valid for ksp d 1), this I is the derivative of the transmitted ini i g 2 g r tensity I = A2r + Asp e−2ksp d + 2Ar Asp e−ksp d cos(ksp d + ϕ0 ) with respect to the magnetic ﬁeld: i Imp = −4Agsp 2 e−2ksp d ksp d 0r 0i i d cos ksp d + ϕ0 − 4Ar Agsp e−ksp d ksp 0r r + ksp d sin ksp d + ϕ0 . 0i (A1) As can be seen, this expression consists of a ﬁrst small offset term, a component in phase with the optical interferogram i associated with ksp , and a π /2-shifted component due r to ksp . Neglecting the offset term, and applying some trigonometry, Eq. (A1) can be expressed as 0i r 2 + k i 2 Imp = −4Ar Agsp e−ksp d d ksp sp 0r × sin ksp d + ϕ0 + φ , (A2) i r where φ is deﬁned as tan φ = ksp /ksp . This φ phase can be determined as the shift between the maxima (or minima) of the optical interferogram and the zeros of the magnetoplasmonic one [see zoom in Fig. 1(b) of the main text]. 035118-6 SPECTRAL DEPENDENCE OF THE MAGNETIC . . . PHYSICAL REVIEW B 86, 035118 (2012) The Imp signal can be normalized by the amplitude contrast of the optical intensity I , Icontrast = 4Ar Asp , resulting in norm r 2 + k i 2 sin k 0r d + ϕ + φ . (A3) Imp = −d ksp 0 sp sp The amplitude of this normalized Imp is then proportional r )2 + (k i )2 × d. By determining the amplitude of to (ksp sp * 19 diana.martin@imm.cnm.csic.es; also at International Iberian Nanotechnology Laboratory, 4710-229 Braga, Portugal. † Now at Institut des Molécules et Matériaux du Mans, UMR CNRS 6283, Université du Maine, 72085 Le Mans cedex, France. ‡ Now at Joint Quantum Institute, National Institute of Standards and Technology and University of Maryland, Gaithersburg, MD, USA. § Now at Institute of Physics, Chemnitz University of Technology, D-09107 Chemnitz, Germany. maria-ujue.gonzalez@csic.es 1 W. L. Barnes, A. Dereux, and T. W. Ebbesen, Nature 424, 824 (2003). 2 E. Ozbay, Science 311, 189 (2006). 3 T. W. Ebbesen, C. Genet, and S. I. Bozhevolnyi, Phys. Today 61(5), 44 (2008). 4 D. K. Gramotnev and S. I. Bozhevolnyi, Nat. Photonics 4, 83 (2010). 5 B. Berini and I. De Leon, Nat. Photonics 6, 16 (2012). 6 A. V. Krasavin, K. F. MacDonald, N. I. Zheludev, and A. V. Zayats, Appl. Phys. Lett. 85, 3369 (2004). 7 T. Nikolajsen, K. Leosson, and S. I. Bozhevolnyi, Appl. Phys. Lett. 85, 5833 (2004). 8 D. Paciﬁci, H. J. Lezec, and H. A. Atwater, Nat. Photonics 1, 402 (2007). 9 R. A. Pala, K. T. Shimizu, N. A. Melosh, and M. L. Brongersma, Nano Lett. 8, 1506 (2008). 10 M. J. Dicken, L. A. Sweatlock, D. Paciﬁci, H. J. Lezec, K. Bhattacharya, and H. A. Atwater, Nano Lett. 8, 4048 (2008). 11 J. A. Dionne, K. Diest, L. A. Sweatlock, and H. A. Atwater, Nano Lett. 9, 897 (2009). 12 K. F. MacDonald, Z. L. Sámson, M. I. Stockman, and N. I. Zheludev, Nat. Photonics 3, 55 (2009). 13 V. V. Temnov, K. Nelson, G. Armelles, A. Cebollada, T. Thomay, A. Leitenstorfer, and R. Bratschitsch, Opt. Express 17, 8423 (2009). 14 J. Gosciniak, S. I. Bozhevolnyi, T. B. Andersen, V. S. Volkov, J. Kjelstrup-Hansen, L. Markey, and A. Dereux, Opt. Express 18, 1207 (2010). 15 V. V. Temnov, G. Armelles, U. Woggon, D. Guzatov, A. Cebollada, A. Garcı́a-Martı́n, J. Garcı́a-Martı́n, T. Thomay, A. Leitenstorfer, and R. Bratschitsch, Nat. Photonics 4, 107 (2010). 16 D. Martı́n-Becerra, J. B. González-Dı́az, V. V. Temnov, A. Cebollada, G. Armelles, T. Thomay, A. Leitenstorfer, R. Bratschitsch, A. Garcı́a-Martı́n, and M. U. González, Appl. Phys. Lett. 97, 183114 (2010). 17 A. Agrawal, C. Susut, G. Stafford, U. Bertocci, B. McMorran, H. J. Lezec, and A. A. Talin, Nano Lett. 11, 2774 (2011). 18 S. Randhawa, S. Lachèze, J. Renger, A. Bouhelier, R. E. de Lamaestre, A. Dereux, and R. Quidant, Opt. Express 20, 2354 (2012). norm r i Imp and φ, we can obtain ksp and ksp . J. J. Brion, R. F. Wallis, A. Hartstein, and E. Burstein, Phys. Rev. Lett. 28, 1455 (1972). 20 K. W. Chiu and J. J. Quinn, Phys. Rev. Lett. 29, 600 (1972). 21 R. F. Wallis, J. J. B. E. Burstein, and A. Hartstein, Phys. Rev. B 9, 3424 (1974). 22 J. B. Khurgin, Appl. Phys. Lett. 89, 251115 (2006). 23 W. V. Parys, B. Moeyersoon, D. V. Thourhout, R. Baets, M. Vanwolleghem, B. Dagens, J. Decobert, O. L. Gouezigou, D. Make, R. Vanheertum, and L. Lagae, Appl. Phys. Lett. 88, 071115 (2006). 24 B. Sepúlveda, L. Lechuga, and G. Armelles, J. Lightwave Technol. 24, 945 (2006). 25 Z. Yu, G. Veronis, Z. Wang, and S. Fan, Phys. Rev. Lett. 100, 023902 (2008). 26 J. Montoya, K. Parameswaran, J. Hensley, M. Allen, and R. Ram, J. Appl. Phys. 106, 023108 (2009). 27 A. V. Kimel, A. Kirilyuk, P. A. Usachev, R. V. Pisarev, A. M. Balbashov, and Th. Raising, Nature (London) 435, 655 (2005). 28 J. B. González-Dı́az, A. Garcı́a-Martı́n, G. Armelles, J. M. Garcı́aMartı́n, C. Clavero, A. Cebollada, R. A. Lukaszew, J. R. Skuza, D. P. Kumah, and R. Clarke, Phys. Rev. B 76, 153402 (2007). 29 E. Ferreiro-Vila, J. B. González-Dı́az, R. Fermento, M. U. González, A. Garcı́a-Martı́n, J. M. Garcı́a-Martı́n, A. Cebollada, G. Armelles, D. Meneses-Rodrı́guez, and E. M. Sandoval, Phys. Rev. B 80, 125132 (2009). 30 C. Clavero, K. Yang, J. R. Skuza, and R. A. Lukaszew, Opt. Express 18, 7743 (2010). 31 E. Ferreiro-Vila, M. Iglesias, E. Paz, F. J. Palomares, F. Cebollada, J. M. González, G. Armelles, J. M. Garcı́a-Martı́n, and A. Cebollada, Phys. Rev. B 83, 205120 (2011). 32 J. Renger, S. Grafström, and L. M. Eng, Phys. Rev. B 76, 045431 (2007). 33 J. B. González-Dı́az, Ph.D. thesis, Universidad Autónoma de Madrid, Spain, 2010. 34 Although this peak has not been experimentally conﬁrmed since the very short plasmon propagation distance at wavelengths below 530 nm has prevented the measurement, the good accord between measurements and simulations in the rest of the spectral range allows us to trust the presence of this peak. 35 S. A. Maier, Plasmonics: Fundamentals and Applications (Springer, Berlin, 2007). 36 P. B. Johnson and R. W. Christy, Phys. Rev. B 6, 4370 (1972). 37 P. B. Johnson and R. W. Christy, Phys. Rev. B 9, 5056 (1974). 38 G. S. Krinchik, J. Appl. Phys. 35, 1089 (1964). 39 E. D. Palik, Handbook of Optical Constants of Solids (Academic Press, San Diego, 1998). 40 K. Mok, G. J. Kovács, J. McCord, L. Li, M. Helm, and H. Schmidt, Phys. Rev. B 84, 094413 (2011). 035118-7